Applications of Hard X-ray
Photoelectron Spectroscopy in
Lee Walsh B.Sc
A thesis presented for the degree of
Doctor of Philosophy
Department of Physical Sciences
Dublin City University
I hereby certify that this material, which I now submit for assessment on the pro-gramme of study leading to the award of doctor of Philosophy is entirely my own work, that I have exercised reasonable care to ensure that the work is original, and does not to the best of my knowledge breach any law of copyright, and has not been taken from the work of others save and to the extent that such work has been cited and acknowledged within the text of my work.
Firstly and most importantly I would like to thank my family and my girlfriend Paula for the help, support (and patience) they have given me throughout my studies. I would like to thank all my friends in Dublin and Maynooth, especially Dervil, Paul and Peter for their friendship, and distraction, throughout the last few years.
I would also like to thank my supervisor Greg Hughes for all of his guidance, or allowing me the room to make my own decisions and mistakes, and especially for making sure we got as many trips away as possible.
I would like to express my gratitude to everyone in DCU: Justin, Anthony, Rob, Barry, Conor, Tom, Rajesh, and Lalit for the help they gave me during the project but in particular for the morning debates, where the issues of the world, and football in particular, were resolved. I would like to thank Pat Wogan for taking the time to answer questions and help with technical issues. I would also like to thank everyone in the Tyndall Institute in Cork: Paul, Sally, Karim and Vladmir for helping me. I would also like to thank Pat Lysaght from SEMATECH for inviting me to get involved with his project, and Joseph Woicik, Dan Fischer and Conan Weiland from NIST who helped massively with getting beamtime and performing experiments.
Publications Arising From This
A spectroscopic method for the evaluation of surface passivation treat-ments on metal-oxide-semiconductor structures
Lee. A . Walsh, Paul K. Hurley, Jun Lin, T.P. O’Regan, Joseph C. Woicik, Greg Hughes
Applied Surface Science 301 (2014) 40.
Hard x-ray photoelectron spectroscopy and electrical characterisation study of the surface potential in metal/Al2O3/GaAs(100)
Lee. A . Walsh, Paul K. Hurley, Jun Lin, T.P. O’Regan, Eric Cockayne, Joseph C. Woicik, Greg Hughes
Physical Review B 88 (2013) 045322.
A combined hard x-ray photoelectron spectroscopy and electrical char-acterisation study of metal/SiO2/Si(100) metal-oxide-semiconductor
Lee. A . Walsh, Paul K. Hurley, Jun Lin, Joseph C. Woicik, Greg Hughes Applied Physics Letters101 (2012) 241602.
A combined capacitance-voltage and hard x-ray photoelectron spec-troscopy characterisation of metal/Al2O3/In0.53Ga0.47As capacitor
Journal of Applied Physics (in process).
Investigation of Ni-InGaAs alloy formation by hard x-ray photoelectron spectroscopy and x-ray absorption spectroscopy
Lee. A . Walsh, Conan Weiland, Joseph C. Woicik, Greg Hughes, Rinus T.P. Lee, Wei-Yip Loh, Patrick Lysaght, Chris Hobbs
HAXPES and electrical characterisation studies of metal-oxide-semiconductor structures on Si and sulphur passivated GaAs (oral presentation)
Lee. A . Walsh, Paul K. Hurley, Jun Lin, T.P. O’Regan, Joseph C. Woicik, Greg Hughes
VIII International Workshop on Semiconductor Surface Passivation, Krakow, Poland (September 2013).
HAXPES and electrical characterisation studies of metal-oxide-semiconductor structures on Si and GaAs (oral presentation)
Lee. A . Walsh, Paul K. Hurley, Jun Lin, T.P. O’Regan, Eric Cockayne, Joseph C. Woicik, Greg Hughes
5th International Conference on Hard X-ray Photoelectron Spectroscopy, Uppsala,
Sweden (June 2013).
Combined HAXPES and electrical characterisation studies of metal-oxide-semiconductor structures on Si and GaAs (poster presentation)
Lee. A . Walsh, Paul K. Hurley, Jun Lin, T.P. O’Regan, Eric Cockayne, Joseph C. Woicik, Greg Hughes
AVS 59th International Symposium and Exhibition, Tampa, USA (October 2012).
HAXPES and electrical characterisation studies of metal-oxide-semiconductor structures on Si and GaAs (poster presentation)
Lee. A. Walsh, B. Brennan, R. M. Wallace, Joseph C. Woicik and Greg Hughes Intel European Research & Innovation Conference, Leixlip, Ireland (October 2011).
structures on InGaAs substrates (poster presentation)
Lee. A . Walsh, Barry Brennan, Robert M. Wallace, Paul K. Hurley, Jun Lin, Joseph C. Woicik, Greg Hughes
4thInternational Conference on Hard X-ray Photoelectron Spectroscopy, Hamburg, Germany (September 2011).
Contents1 Introduction 1 1.1 History . . . 1 1.2 Applications of HAXPES . . . 5 1.2.1 Chemical Studies . . . 5 1.2.2 Electronic Structure . . . 6
1.2.3 Combination of HAXPES and Other Techniques . . . 7
1.2.4 Other Work . . . 8
1.3 III-V MOSFET Issues . . . 10
1.3.1 A Suitable Dielectric Material . . . 12
1.3.2 Lattice Matching to Si . . . 13
1.3.3 Low Dit High-κ/Semiconductor Interface . . . 14
1.3.4 Source/Drain Contact Material . . . 15
1.4 Thesis Layout and Organisation . . . 17
2 Theory and Experimental Techniques 32 2.1 X-ray Photoelectron Spectroscopy . . . 32
2.1.1 Theoretical Basis . . . 32
2.1.2 Referencing of Binding Energy . . . 34
2.1.3 Initial and Final State Effects . . . 36
2.1.4 Peak Widths . . . 37 2.1.5 Sampling Depth . . . 38 2.1.6 Element Identification . . . 39 2.1.7 Chemical Shift . . . 40 2.1.8 Peak Fitting . . . 41 2.1.9 Apparatus . . . 42 2.1.10 System Used . . . 47
2.2 Hard X-ray Photoelectron Spectroscopy . . . 48
2.2.1 Advantages of HAXPES . . . 48
2.2.2 Apparatus . . . 49
2.2.3 Systems Used . . . 54
2.3 X-ray Absorption Spectroscopy . . . 55
2.3.1 Theory . . . 55 2.3.2 Data Analysis . . . 61 2.3.3 Apparatus . . . 61 2.3.4 Systems Used . . . 63 2.4 Capacitance-Voltage Profiling . . . 64 2.4.1 Theory . . . 64
3 Initial Investigations of the Measurement Capabilities of
3.1 Introduction . . . 73
3.2 Experimental Details . . . 77
3.3 Results and Discussion . . . 81
3.3.1 Energy Resolution as a Function of Photon Energy . . . 81
3.3.2 Investigation of Sampling Depth . . . 83
3.3.3 Al-Silicide Study at the Al/SiO2 Interfaces . . . 86
3.3.4 HAXPES Characterisation of HfO2/InGaAs Based MOS Struc-tures . . . 90
3.3.5 Photon Energy Drift . . . 95
3.3.6 A Combined HAXPES and Electrical Characterisation Study of SiO2/Si(100) Based MOS Structures . . . 97
3.3.7 Forming Gas Anneal Attempts . . . 107
3.4 Chapter Conclusion . . . 113
4 Combined HAXPES and C-V Characterisation of III-V Based MOS Structures 119 4.1 Introduction . . . 119
4.2 Experimental Details . . . 122
4.3 Results and Discussion . . . 125
4.3.1 Al2O3/GaAs(100) Based MOS Structures . . . 125
4.3.2 Al2O3/In0.53Ga0.47As Based MOS Structures . . . 137
5 Novel salicide materials for source/drain regions in InGaAs
5.1 Introduction . . . 158
5.2 Experimental Details . . . 161
5.3 Results and Discussion . . . 163
5.3.1 Ni-InGaAs . . . 163
5.3.2 Mo-InGaAs . . . 181
5.4 Conclusion . . . 188
6 Conclusions and Future Work 197 6.1 Conclusions . . . 197
6.2 Future work . . . 199
6.2.1 HAXPES measurements of in-situ biased samples . . . 199
List of Figures
1.1 Dependence of inelastic mean free path on photon energy . . . 3
1.2 Dependence of photoionisation cross section on photon energy . . . 4
1.3 HAXPES publications per year . . . 5
1.4 Schematic diagram of an n-MOSFET . . . 10
1.5 Evolution of the number of transistors per chip . . . 11
1.6 Cross-section of InGaAs integrated onto a Si substrate by means of buffer layers . . . 13
1.7 Illustration of the direct wafer bonding technique used to produce InGaAs on Si wafers . . . 14
1.8 Illustration of the ion implantation of Si MOSFET to form self-aligned source/drain regions . . . 15
2.1 Photoelectric effect . . . 33
2.2 Energy level diagram of XPS sample . . . 35
2.3 Exponential nature of XPS signal . . . 39
2.4 Survey scan of Al sample . . . 40
2.5 SiO2 chemical shift . . . 41
2.7 Hemispherical analyser . . . 45
2.8 Channel plate . . . 46
2.9 XPS experimental set-up . . . 46
2.10 Conventional XPS system. . . 47
2.11 HAXPES survey scans . . . 49
2.12 Depth profile of HfO2/SiO2/Si sample . . . 50
2.13 Synchrotron radiation source . . . 51
2.14 Undulator diagram. . . 52
2.15 Double crystal monochromator . . . 54
2.16 HAXPES experimental setup . . . 55
2.17 Simple XAS spectra . . . 57
2.18 XAS process . . . 58
2.19 Grazing incidence XAS . . . 60
2.20 Reflectivity curve for XAS . . . 60
2.21 XAS experimental setup . . . 62
2.22 XAS system . . . 63
2.23 Energy band diagram for an ideal p-type MOS capacitor . . . 65
2.24 Accumulation in a p-type MOS . . . 66
2.25 Depletion in a p-type MOS . . . 67
2.26 Inversion in a p-type MOS . . . 68
3.1 SiO2/Si samples for HAXPES and C-V characterisation . . . 79
3.2 Normalised Si 2p spectra acquired at a range of photon energies . . 82 3.3 Normalised Al 1s spectra acquired at a range of photon energies . . 82 3.4 Fitted Ni Fermi edge spectrum . . . 83 3.5 Survey spectra of Al/SiO2/Si samples acquired at a range of photon
energies . . . 84 3.6 Normalised Al 1s spectra demonstrating the dependence of
sam-pling depth on photon energy . . . 85 3.7 Normalised Si 1s spectra of Al-silicide samples at a range of anneal
temperatures . . . 87 3.8 Normalised Al 1s spectra of Al-silicide samples at a range of anneal
temperatures . . . 88 3.9 Normalised Si 2p spectra of Al-silicide samples at a range of anneal
temperatures, acquired at 4150 eV . . . 89 3.10 Normalised Si 1s spectra of Al-silicide samples at a range of anneal
temperatures, acquired at 2140 eV . . . 89 3.11 Al-silicide sample structure . . . 90 3.12 TEM images of HfO2/InGaAs samples . . . 92
3.13 Normalised As 2p core level spectra acquired at a photon energy of 4150 eV for the uncapped, Pt and Al capped HfO2/InGaAs samples 93
3.14 Normalised valence band spectra of uncapped, Al, and Pt capped HfO2/InGaAs MOS structures on n-InGaAs. . . 94
3.15 Photon energy drift . . . 97 3.16 Normalised Si 1s core level spectra acquired at a photon energy of
4150 eV for the uncapped SiO2/Si, Ni (5 nm) capped SiO2/Si, and
3.17 Valence band spectra of an n-type SiO2/Si sample . . . 100
3.18 Band diagram for uncapped, Al and Ni capped SiO2/p-Si sample . 103
3.19 C-V characteristics (1 MHz) for the metal/SiO2/Si samples . . . 105
3.20 Multi-frequency (1 kHz - 1 MHz) C-V characteristics for n and p-Si samples . . . 106 3.21 Multi-frequency (1 kHz - 1 MHz) C-V characteristics for n and p-Si
samples following post-metallisation FGA. . . 109 3.22 Normalised spectra of the Ni 2p spectra before and after
post-metallisation FGA. . . 110 3.23 Normalised Si 1s core level spectra for the 3 hour pre-metallisation
uncapped, Al and Ni capped SiO2/Si samples. . . 111
3.24 100 kHz C-V characteristics for n and p-Si samples following a 3 hour pre-metallisation FGA . . . 112 4.1 InGaAs and GaAs samples for HAXPES and C-V characterisation . 123 4.2 Normalised As 2p core level spectra acquired at a photon energy of
4150 eV for the uncapped Al2O3/GaAs, Ni (5 nm) capped and Al
(5 nm) capped Al2O3/GaAs samples . . . 126
4.3 Total theoretical DOS, convolved cross-section weighted DOS and experimental photoemission valence band spectra of n-GaAs/Al2O3 128
4.4 Simulation of the band-bending in a p-type GaAs MOS structure . 129 4.5 Multi-frequency (1 kHz to 1 MHz) C-V responses Al2O3/GaAs based
MOS structures . . . 131 4.6 1 MHz C-V for Al and Ni gate on Al2O3/GaAs MOS structures . . 132
4.8 Al 1s spectra showing BE shift due to the changes in the potential
across the Al2O3 layer caused by different workfunction metals . . . 136
4.9 Band diagram, illustrating the BE shifts due to an electric field across the oxide caused by metal deposition for p-GaAs . . . 138
4.10 Normalised and fitted As 2p core level spectra acquired at a photon energy of 4150 eV for the uncapped, Ni (5 nm) capped, and Al (5 nm) capped Al2O3/InGaAs samples . . . 139
4.11 Valence band spectra of an n-type Al2O3/InGaAs sample . . . 141
4.12 Band diagrams of unmetallised, Al and Ni capped Al2O3/InGaAs MOS structures . . . 142
4.13 C-V responses at 1 MHz Al gate and Au/Ni gate over Al2O3/InGaAs145 4.14 HR-TEM images of the Al2O3/InGaAs based MOS capacitors . . . 146
4.15 Al 1s spectra showing BE shift due to the changes in the potential across the Al2O3 layer . . . 149
5.1 NiInGaAs formation process . . . 160
5.2 Sheet resistance measurements for Ni-InGaAs samples . . . 164
5.3 SEM and TEM images of 5 nm Ni capped samples . . . 165
5.4 Normalised and fitted In 3d, As 2p, and Ga 2p HAXPES spectra acquired at a photon energy of 2200 eV for a SiN/InGaAs sample . 167 5.5 Normalised Si 1s spectra for the SiN capping layer . . . 168
5.6 Normalised and fitted Ni 2p HAXPES spectra for SiN-Ni-InGaAs samples . . . 169
5.7 Normalised and fitted Ga 2pHAXPES spectra, and Ga K-edge XAS spectra for SiN-Ni-InGaAs samples . . . 171
5.9 Normalised and fitted As 2p HAXPES spectra and As K-edge XAS spectra for SiN-Ni-InGaAs samples . . . 175 5.10 Normalised and fitted As 3d HAXPES spectra for SiN-Ni-InGaAs
samples . . . 177 5.11 Normalised and fitted Ga 2p spectra and In 3d spectra for
SiN-Ni-InGaAs samples acquired at 2200 and 3000 eV photon energy. . . . 178 5.12 Plots of the normalised HAXPES peak areas as a function of
tem-perature . . . 179 5.13 Ni-InGaAs flow chart . . . 181 5.14 Schematic diagram showing the deduced Ni-InGaAs sample structure182 5.15 Normalised and fitted As 2p HAXPES spectra for SiN-Ni-InGaAs
samples acquired at 3000 eV . . . 183 5.16 Normalised and fitted As 2p HAXPES spectra for SiN-Ni-InGaAs
samples acquired at 4000 eV . . . 183 5.17 Normalised and fitted Ga 2p HAXPES spectra for SiN-Ni-InGaAs
samples acquired at 3000 eV . . . 184 5.18 Normalised and fitted Ga 2p HAXPES spectra for SiN-Ni-InGaAs
samples acquired at 4000 eV . . . 185 5.19 Normalised and fitted In 3d HAXPES spectra for SiN-Ni-InGaAs
samples acquired at 3000 eV . . . 186 5.20 Normalised and fitted In 3d HAXPES spectra for SiN-Ni-InGaAs
samples acquired at 4000 eV . . . 187 5.21 Normalised and fitted Mo 3d HAXPES spectra for SiN-Ni-InGaAs
samples acquired at 3000 eV . . . 188 5.22 Schematic diagram showing the deduced Mo-InGaAs sample structure189
6.2 Band diagram of MOS structure with and without an applied
pos-itive bias voltage (Fermi level movement only) . . . 201
6.3 Band diagram of MOS structure with and without an applied pos-itive bias voltage (interface charge only) . . . 202
6.4 Ga 2p peaks of GaAs samples with applied bias . . . 203
6.5 Ga 2p peak position as a function of applied bias voltage . . . 204
List of Tables
1.1 Band gaps and mobilities of Si and III-V materials . . . 12 3.1 SiO2/Si samples for HAXPES analysis . . . 79
3.2 Summary of the HAXPES and C-V results for SiO2/Si samples . . 106
3.3 Summary of the HAXPES results for 3 hour pre-metallisation FGA samples . . . 112 4.1 Comparison of Fermi level positions recorded by HAXPES and C-V
measurements in Al2O3/GaAs based MOS structures . . . 135
4.2 Comparison of the calculated and measured shifts in the Al oxide peak due to the presence of a potential field across the oxide layer. . 136 4.3 Surface Fermi level positions obtained from C-V analysis HAXPES
measurements for uncapped, Al gate and Ni gate Al2O3/InGaAs
Applications of Hard X-ray Photoelectron Spectroscopy in
Semiconductor Materials Characterisation
The recently developed high energy variant of x-ray photoelectron spectroscopy (XPS), known as hard x-ray photoelectron spectroscopy (HAXPES), has been used to study various semiconductor material systems. Extending the photoemission sampling depth to>10 nm into the material surface by the use of monochromatic x-ray photons in the 2 to 4 keV energy range, enables the acquisition of chemi-cal and electronic information deeper into the bulk than is possible with conven-tional XPS, and facilitates the investigation of multilayer structures. In this study, combined HAXPES and electrical characterisation studies were performed on Si, GaAs and InGaAs based metal-oxide-semiconductor (MOS) structures in order to cross-correlate the electronic information derived from these different measure-ment methods. The results obtained indicate that surface potential changes at the semiconductor/dielectric interface due to the presence of different work function metals can be detected using HAXPES measurements. Changes in the semiconduc-tor band bending at zero gate voltage and the flat band voltage values derived from capacitance-voltage (C-V) measurements are in agreement with the semiconductor core level shifts measured from the HAXPES spectra. Experiments have been per-formed which utilise the increased sampling depth of HAXPES to chemically and structurally characterise Ni-InGaAs and Mo-InGaAs interface formation. These material systems are of interest as possible source drain contacts for use in future high mobility InGaAs based MOS field-effect-transistors due to their extremely low contact resistance and self-aligned formation. Complementary x-ray absorp-tion spectroscopy (XAS) measurements were used in combinaabsorp-tion with HAXPES data to develop a model of the chemical interactions and compound formation at the Ni-InGaAs and Mo-InGaAs interfaces as a function of anneal temperature.
The focus of this thesis is to investigate the potential applications of the high energy variant of x-ray photoelectron spectroscopy (XPS), known as hard x-ray photoelectron spectroscopy (HAXPES). In this section HAXPES will be discussed in relation to the following: 1) the growth of HAXPES since its initial development and 2) the advantages of HAXPES over conventional XPS in regards to the open questions in III-V metal oxide semiconductor field effect transistor (MOSFET) technologies.
The discovery and subsequent explanation of the photoelectric effect by J.J. Thomp-son, and ultimately Albert Einstein, led to the theoretical and experimental basis upon which XPS was founded.1 The first experiments using this basis were
per-formed by Robinson and Rawlin in 1914. They perper-formed simple studies of gold surfaces, using photographic plates, and observed energy spectra.2 X-ray Pho-toelectron Spectroscopy truly began to be used as an analytical technique in its own right in the 1950’s, following development by Steinhardt and Serfass.3 Their initial experiments involved using XPS to determine elemental quantities present
Further development of the technique was performed by Kai Siegbahn, and his group in Uppsala, Sweden.5, 6 In order to use XPS to accurately obtain chemical
information of a surface, it was recognised by Siegbahn that the energy resolution needed to improve. He developed an analyser capable of 1 eV resolution, where resolution had been 3 eV up to that time.7, 8 Using this analyser and a Cu Kα
source (8 keV) sufficiently sharp spectra were produced to allow chemical analysis of the surfaces being studied.7 It was at this time that ultra high vacuum (UHV)
vessels began to be used, as it was appreciated that surface contamination played a large role in the quality and accuracy of the acquired spectra. In addition B.L. Henke’s invention of the hemispherical analyser allowed the use of lower energy dedicated XPS sources.9
XPS proved to be a powerful technique in the chemical analysis of surfaces. However, almost every physical property changes at the surface due to a break in the material symmetry and this leads to surface reconstruction effects which result in differing surface and bulk characteristics. Looking at the change in the inelastic mean free path (IMFP) of photoemitted electrons with kinetic energy, as seen in figure 1.1, it is clear that in order to increase the sampling depth of XPS there were two options: use very low or very high photon energies and correspondingly drastically increase or decrease the photoelectron kinetic energies.10 Low photon energy XPS has been achievable at synchrotron sources for a long time, however there are significant drawbacks.11 The very low photon energy means very few core levels are excited and thus valence band measurements are the primary ap-plication. Additionally, final state effects have an increased influence, leading to an increase in background signal. The use of increased photon energies was first attempted by Pianetta and Lindau in 1974.12 It was realised that an increase of
the sampling depth from 5-7 nm to 10+ nm would be very useful, especially as thin film deposition techniques had not yet been optimised. At that time, the sig-nal intensity for peaks originating from >5 nm had low counts and poor signal to noise, due to the rapid decrease in sub-shell photoionization cross-sections with an increase in photon energy,13 as shown in figure 1.2. Indeed, the early XPS studies by Siegbahn et. al7 were performed using hard x-ray sources, such as Cu Kα (8 keV). However the photon energy was reduced, due to the previously mentioned
Figure 1.1: Diagram shows the increase in IMFP with increasing photon energy14 signal to noise issue as well as an enhanced interest in the sample surface. In recent times the structures used in conventional MOSFET devices have become increas-ingly complex so it has become more desirable to characterise samples close to actual devices, as opposed to the model interfaces which have been conventionally measured.
While these experimental issues halted the use of HAXPES in the years fol-lowing, numerous groups have revived interest in the technique since 2003. The development of purpose-built hard x-ray spectrometers and third generation syn-chrotron radiation sources has allowed for the re-emergence of HAXPES. Third generation synchrotron sources are optimised for brilliance (photon flux per unit area) through the use of insertion devices. The high photon flux (1011 photons/s) achievable with these third generation sources allows the reduction in photoionisa-tion cross-secphotoionisa-tion to be overcome, while the tunable nature of synchrotron sources
Figure 1.2: Dependence of photoionisation cross section on photon energy15 in development at Diamond Synchrotron. Whereas previous measurements of mul-tilayered structures had been performed by techniques such as secondary ion mass spectrometry or cross-sectional transmission electron microscopy (TEM), where destructive sample preparation is involved, HAXPES measurements have the ad-vantage of being non-destructive. There are currently HAXPES ready beamlines at DESY and BESSY in Germany,16, 17 SPring8 in Japan,18 Brookhaven National
Laboratory in the USA,19 Diamond in the UK, and the ESRF in France where
Applications of HAXPES
The increase in, and the tunability of, the sampling depth of HAXPES performed at synchrotron sources has led to an expanded field of application. Figure 1.3 shows the increase in publications containing HAXPES measurements in recent years. The large growth seen in the past five years is primarily due to the increase in HAXPES-ready beamlines. This section will give a brief overview of the areas of research in which HAXPES has been employed. The areas of research have been split into four groups: 1) chemical studies, 2) electronic structure, 3) HAXPES as a complementary technique, and 4) other studies.
Figure 1.3: Number of HAXPES publications in recent years taken from Web of Knowledge,22 as of 30/6/14.
ma-of HAXPES is, therefore, the chemical characterisation ma-of the surface and bulk ma-of materials, or the interfaces in the case of multi-layered structures. These studies have varied from investigating the chemical bonds present at reactive interfaces to investigating the loss of certain materials during the course of an anneal study. The majority of the work has followed the general trend of materials research in recent years, in that it focusses on applied materials for specific technological purposes.
The depth profiling capability of HAXPES has enabled the non-destructive depth profiling of a number of systems, from the investigation of the chemical composition of passive oxide films on stainless steel,23 to the study of nitrogen
in-corporation in HfO2 and SiO2 films for use in advanced MOSFET devices.24 The
ability to investigate the chemical composition of buried interfaces in multilayer structures has found use in the characterisation of the Fe3O4/InAs interface (a
pro-totypical system for spin injection electrodes in spintronic devices25), complex
Ge-based multilayer devices,26 and thick (>10 nm) Cr-O-Al films on Si substrates.27
HAXPES has also been used to investigate a variety of devices with specific applica-tions including: substrate and oxide materials to replace the conventional SiO2/Si
system for future MOSFETs,28, 29 organic and conventional semiconductor-based
solar cells,30–35 ferromagnetic materials for use in spintronics,36–41 exotic oxide
materials for use in fuel cells,42 materials with superconducting properties,43, 44 in-terface composition and degradation during cycling in batteries,45, 46 and material systems for use in non-volatile memory.47, 48
Conventional XPS has been previously used to derive some information on the electronic structure of materials. The surface sensitive nature of the technique is one of it’s strengths, however, the ability to probe the material bulk would extend it’s applications, as the electronic structure at the surface of a material is vastly different to the bulk behaviour, due to the break in symmetry.14 The bulk sensitive nature of HAXPES adds this functionality.
in semiconductor based structures, as not only can the Fermi level position in the bulk of the material be evaluated but, due to the tunable nature of synchrotron based HAXPES work, the sampling depth can be varied, allowing for the profile of the band-bending to be measured.40, 47 The ability to accurately evaluate the Fermi level position, conduction band minimum, and valence band maximum also allows for the accurate evaluation of electron band line-up and the creation of band offset diagrams,30, 32, 43, 49, 50 which are important in determining device
per-formance. Measurement of the valence band edge of a given material or structure also allows for the density of states to be extracted, which can give information on the conductivity and ferromagnetic properties.34, 50, 51 HAXPES measurements of
magnetized samples have also been performed byKozina et. al52in order to
mea-sure circular magnetic dichroism in materials for use in spintronics. This approach involves the use of a phase retarder which the x-ray beam passes through prior to interaction with the sample, and the difference in peak intensity measured at each polarisation allows the circular magnetic dichroism to be evaluated.
Combination of HAXPES and Other Techniques
As the above sections have demonstrated, HAXPES has proven to be very useful in the chemical and electrical characterisation of the material bulk and buried interfaces. Numerous groups realised that it could be even more useful when combined with other techniques in order to gain a more complete understanding of a given sample. This is more than simply performing two techniques on the same sample. It involves choosing an appropriate technique to complement HAXPES for a given sample set.
HAXPES has been combined with x-ray diffraction (XRD) byRubio-Zuazo et. al in order to study the magnetic and transport properties of strongly correlated electron systems.53 XRD is sensitive to atomic structure and the ability to perform both measurements simultaneously on the same sample helps to fully explain the macroscopic behaviour of the studied system. Anniyev et. al combined HAXPES
provides useful information as to the reactivity of the catalyst in question.54 While
HAXPES probes the occupied electronic states, XAS probes the unoccupied va-lence states. Similar complementary experiments have been performed combining HAXPES with standing wave XPS,55 and x-ray reflectivity measurements.26
Certain applications of HAXPES, while fitting into either electronic or chemical characterisation, are unique enough to belong in a section of their own. This section discusses such experiments. The ability to non-destructively investigate chemical and electronic properties of materials has positioned HAXPES uniquely in the field of materials science research. As such, it has found applications in the study of the fundamental physical, and electronic properties of various material systems which have been beyond the measurement capabilities of current techniques.
An area which has seen a large publication increase in the last few years is the study of the electron correlation effects present within various exotic oxide materials. Electron correlation simply describes the fact that the behaviour of an individual electron in a material system is not independent of all other electrons, as assumed by the Hartree-Fock approximation. Strongly correlated materials exhibit unusual electronic and magnetic behaviour, some of which is useful in certain applications such as spintronics and Mott insulators. HAXPES has been very useful in the analysis of these correlated materials due to the ability to probe structural, electronic and magnetic properties at a variety of sampling depths into the material. Grebinskij et. al56 have investigated the correlation effects
present in SrRuO3, a ferromagnetic metallic oxide which is popular as an electrode
material due to its good electrical conductivity and chemical stability. Previous attempts to measure the correlation effects present in this system with techniques such as resonant photoemission spectroscopy have been unsuccessful, however, the application of angularly resolved HAXPES was used to measure the valence bands and identify SrRuO3 as a weakly correlated material. Suga et. al57 have used the
ability to tune the photon energy, and thus the sampling depth, to characterise both the bulk electronic structure of VO2, known to display correlation effects,
and the surface of the material where the electronic structure displays different behaviour.
The Kondo effect was first observed in the 1930’s58 and fully explained in the 1960’s,59 however, the fabrication and measurement techniques available did not
allow for sufficiently controlled measurement of these systems. Kondo systems are metal compounds in which the conduction electrons are scattered, due to magnetic impurities in the material. Whereas normal metals display a decrease in resistivity with decreasing temperature, these Kondo systems actually show an increase in resistivity at very low temperatures. The bulk sensitivity of HAXPES has allowed researchers to analyse the electronic structure of Kondo systems such as YbNi3X9,60 YbAl2,61 YbCu2Si2,62 YbB12 and SmB6.63
III-V MOSFET Issues
The progress in metal oxide semiconductor (MOS) transistor technology, as shown in figure 1.4, which has continued unhindered since the initial development by Kahng and Atalla for Bell labs in 1959,64 is currently reaching a crossroads. The
downscaling of the Si channel width, which has increased the number of transis-tors, as seen in figure 1.5, and thus the power density, on a chip, according to Moore’s Law,65 is reaching a stage at which quantum tunnelling effects will begin
to dominate. Previous issues such as the limit of the dielectric thickness have been addressed by the application of high-κ materials,66 which enable higher drive currents and thus increased output power from the device, while also reducing the leakage current, resulting in improved efficiency.
Figure 1.4: Schematic diagram of an n-MOSFET
The continued scaling of MOSFET devices, as described by the International Technology Roadmap for Semiconductors,68 beyond the 16 nm node, where 16 nm
is the metal 1 half-pitch, necessitates an alternative channel material in order to continue the improvement in performance and efficiency. The prime candidates for replacing Si as the channel material in n-MOS are the III-V family of compound
Si GaAs In0.53GaAs0.47 InP
Eg (eV) 1.12 1.42 0.75 1.35
µe (cm2/Vs) 800 4000 7000 3200
Table 1.1: Band gap and mobility for Si and III-V materials69
semiconductors, in particular GaAs, InP, and InGaAs, while Ge is the likely ma-terial for use in p-MOS. As is clear from table 1.1, all three provide significant gains in electron mobility over Si, which in turn should result in faster transistors. In0.53Ga0.47As has recently emerged as the most promising of the III-V materials
for integration into n-MOS devices. The 53 % In and 47 % Ga concentrations are used as this particular composition is lattice matched to InP, which is a cheap semiconductor material on which the InGaAs devices can be grown. There are however a number of remaining issues which need to be resolved before InGaAs can be integrated into MOSFET processing:
1. The need for a suitable dielectric material. 2. A method for lattice matching InGaAs to Si.
3. Achieving a suitably low density of defect states for the high-κ/III-V inter-face.
4. The need for a source/drain contact material.
A Suitable Dielectric Material
While Si was a fortuitous material, in that both Si and its native oxide (SiO2)
perform well electrically and have naturally low levels of defect states at the inter-face, the same cannot be said for InGaAs. The native oxides of InGaAs have very poor electrical characteristics and as such the need for a replacement dielectric is evident.70 Intensive research into an appropriate dielectric has highlighted atomic
layer deposited (ALD) Al2O3,71, 72 ZrO273, 74 and HfO275, 76to be the leading
involved lead to a ’self-cleaning’ effect which removes the native oxide present at the dielectric/InGaAs interface.75, 77, 78
Lattice Matching to Si
The importance of finding a channel material which is lattice matched to Si stems from the fact that the entire semiconductor industry is designed to produce Si transistors. As such finding a material which can be lattice matched to, and thus grown on, Si substrates requires a much smaller evolution from the current growth facilities in the transition from Si to InGaAs based MOSFETs. While InGaAs itself is not lattice matched to Si, a number of approaches have been developed which involve using buffer layers to gradually alter the lattice properties from those of InGaAs to those of Si as shown in figure 1.6,79, 80 however the thickness of the buffer layers required restricts the downscaling of the InGaAs MOSFET. An alternative method involves the direct wafer bonding of III-V and Si substrates, as shown in figure 1.7, which has the advantage of better quality and thinner III-V layers on Si.81, 82
Figure 1.7: Illustration of the direct wafer bonding technique used to produce InGaAs on Si wafers.82
The greatest issue currently facing InGaAs MOSFET integration is the high den-sity of defect states (Dit) at the high-κ/InGaAs interface. The high Dit arises
due to a multitude of issues including the presence of dangling bonds, dimers and native oxides at the semiconductor surface.84–87 High D
it results in a restricted, or
in extreme cases, pinned Fermi level which hampers MOSFET device operation.88
To overcome these issues a number of passivation treatments have been developed; from wet chemical passivation treatments such as (NH4)2S,85, 89, 90 interface
con-trol layers,91–93 and forming gas (H2N2) anneals,94 with varying degrees of success.
There remains an issue in the evaluation of the electrical characteristics of high Dit
interfaces, as conventional electrical techniques, such as capacitance-voltage (C-V) profiling, find it difficult to extract definitive information in these cases. The large
characteristic response time of the defects involved mean methods such as C-V can only measure small portions of III-V bandgaps.95 HAXPES may provide an
independent method of evaluating the electrical behaviour of these systems, and may also be able to energy map the interface states across the whole bandgap.
Source/Drain Contact Material
Self-aligned source/drain (S/D) contacts in Si MOSFETs have traditionally been formed by taking, for example, a p-type Si substrate and preferentially doping certain regions with n-type dopants using ion implantation; heavy doping is used to decrease sheet resistivity. These regions act as the S/D in the Si MOSFET as schematically shown in figure 1.8. The self-aligned aspect refers to the manufac-turing process. S/D formation involves ion implantation after the formation of the gate stack on the Si substrate; subsequent thermal annealing results in the activa-tion of the Si dopants. The advantage of this process is the formaactiva-tion of the S/D in controlled regions either side of the gate stack, with minimal overlap between the S/D regions and gate contact, and thus a minimal parasitic capacitance.96, 97
Figure 1.8: Illustration of the ion implantation of Si MOSFET to form self-aligned source/drain regions
(salicide) material is a possible solution. Ni-InGaAs has been the most intensively investigated of these materials, displaying excellent sheet resisitivities and the formation of an abrupt interface with InGaAs.99–102 There is, however, still a limited understanding of the formation processes and bonding structures involved. HAXPES could be very useful in addressing this gap in the literature, as the ability to perform depth profiles could help understand both the chemical and structural composition of the Ni-InGaAs layer.
Thesis Layout and Organisation
Chapter 2 describes the chemical, physical and electrical analysis techniques used in this study, along with the principles behind their operation. The primary tech-nique used in this work is HAXPES, however other techtech-niques such as conventional XPS, XAS, and C-V profiling were also used and are discussed.
Chapter 3 describes the initial HAXPES experiments performed in order to un-derstand the capabilities of the technique and equipment. The extended sampling depth and photon energy tunability are demonstrated along with their application in the study of Al-silicide formation in Al/SiO2/Si structures. Combined
HAX-PES and C-V measurements on HfO2/InGaAs are detailed along with the photon
energy drift issue encountered. Successful application of the combined HAXPES and C-V measurements to the model SiO2/Si MOS structure using high and low
workfunction metals are discussed which demonstrate the ability of HAXPES to measure surface Fermi level movements. Finally, attempts at the characterisation of SiO2/Si MOS structures following forming gas anneal are discussed.
Chapter 4 focuses on the extension of the combined HAXPES and C-V charac-terisation method to InGaAs and GaAs based metal oxide semiconductor (MOS) structures. The ability of HAXPES to allow the extraction of Fermi level positions and oxide potential fields is demonstrated on both substrates. C-V measurements of both sample sets are also described and very good agreement between HAXPES and C-V measurements is demonstrated.
Chapter 5 presents an investigation of the Ni-InGaAs and Mo-InGaAs salicide for use as future S/D regions in InGaAs n-MOSFETs. HAXPES, XAS, TEM, and sheet resistivity measurements show the evolution of the chemical, structural, and electrical properties of the salicide throughout the course of an anneal study. The need for the combined application of XAS and HAXPES to fully determine chemical speciation and sample structure is highlighted, and this approach is used to develop a structural and chemical compositional model of the Ni-InGaAs system as it evolves over a thermal annealing range of 250 to 500 ◦C.
1A. Einstein. ¨Uber einen die erzeugung und verwandlung des lichtes betreffenden
heuristischen gesichtspunkt. Annalen der Physik, 322(6):132148, 1905.
2H. Robinson and W. F. Rawlinson. XXXIII. the magnetic spectrum of theβrays
excited in metals by soft x-rays. Philosophical Magazine Series 6, 28(164):277– 281, 1914.
3Ralph Steinhardt and Earl Serfass. X-ray photoelectron spectrometer for
chem-ical analysis. Analytical Chemistry, 23(11):1585–1590, November 1951.
4John C. Vickerman and Ian Gilmore. Surface Analysis: The Principal
Tech-niques. Wiley, March 2009.
5Carl Nordling, Evelyn Sokolowski, and Kai Siegbahn. Precision method
for obtaining absolute values of atomic binding energies. Physical Review, 105(5):1676–1677, March 1957.
6S. Hagstr¨om, C. Nordling, and K. Siegbahn. Electron spectroscopy for chemical
analyses. Physics Letters, 9(3):235–236, April 1964.
7K. Siegbahn, D. Hammond, H. Fellner-Feldegg, and E. F. Barnett. Electron
spectroscopy with monochromatized x-rays. Science, 176(4032):245–252, April 1972.
8K. Siegbahn. Electron spectroscopy for chemical analysis. In Stephen J. Smith
and G. K. Walters, editors, Atomic Physics 3, pages 493–522. Springer US, January 1973.
9B.L. Henke, E.M. Gullikson, J. Kerner, A.L. Oren, and R.L. Blake. Design
and characterization of x-ray multilayer analyzers for the 50-1000 eV region.
Journal of X-Ray Science and Technology, 2(1):17–80, March 1990.
10A. Sekiyama, T. Iwasaki, K. Matsuda, Y. Saitoh, Y. nuki, and S. Suga. Probing
bulk states of correlated electron systems by high-resolution resonance photoe-mission. Nature, 403(6768):396–398, January 2000.
11Herman Winick. Synchrotron radiation research. Plenum Press, 1980.
12I. Lindau, P Pianetta, S Doniach, and W. E. Spicer. X-ray photoemission
spectroscopy. Nature, 250:214–215, July 1974.
13H. Kobayashi, Y. Yamashita, Y. Nakato, T. Komeda, and Y. Nishioka. Interface
states at ultrathin oxide/Si(111) interfaces obtained from x-ray photoelectron spectroscopy measurements under biases.Applied Physics Letters, 69(15):2276– 2278, October 1996.
14Giancarlo Panaccione and Keisuke Kobayashi. Hard x-ray photoemission
spec-troscopy: Variable depth analysis of bulk, surface and interface electronic prop-erties. Surface Science, 606(34):125–129, February 2012.
15J.R. Rubio-Zuazo and G.R. Castro. Hard x-ray photoelectron spectroscopy
(HAXPES) (15 keV) at SpLine, the spanish CRG beamline at the ESRF. Nu-clear Instruments and Methods in Physics Research Section A: Accelerators, Spectrometers, Detectors and Associated Equipment, 547(1):64–72, July 2005.
16Sari Granroth, Weine Olovsson, Erik Holmstrm, Ronny Knut, Mihaela Gorgoi,
Svante Svensson, and Olof Karis. Understanding interface properties from high kinetic energy photoelectron spectroscopy and first principles theory. Journal of Electron Spectroscopy and Related Phenomena, 183(13):80–93, January 2011.
17J. Strempfer, S. Francoual, D. Reuther, D. K. Shukla, A. Skaugen, H.
Schulte-Schrepping, T. Kracht, and H. Franz. Resonant scattering and diffraction beam-line P09 at PETRA III. Journal of Synchrotron Radiation, 20(4):541–549, May
18Y. Takata, M. Yabashi, K. Tamasaku, Y. Nishino, D. Miwa, T. Ishikawa, E.
Ike-naga, K. Horiba, S. Shin, M. Arita, K. Shimada, H. Namatame, M. Taniguchi, H. Nohira, T. Hattori, S. Sdergren, B. Wannberg, and K. Kobayashi. De-velopment of hard x-ray photoelectron spectroscopy at BL29XU in SPring-8.
Nuclear Instruments and Methods in Physics Research Section A: Accelerators, Spectrometers, Detectors and Associated Equipment, 547(1):50–55, July 2005.
19C. Weiland, A.K. Rumaiz, P. Lysaght, B. Karlin, J.C. Woicik, and D.
Fis-cher. NIST high throughput variable kinetic energy hard x-ray photoelectron spectroscopy facility.Journal of Electron Spectroscopy and Related Phenomena.
20Jrg Zegenhagen, Blanka Detlefs, Tien-Lin Lee, Sebastian Thiess, Helena Isern,
Lucien Petit, Lionel Andr, Jrme Roy, Yanyu Mi, and Isabelle Joumard. X-ray standing waves and hard x-ray photoelectron spectroscopy at the insertion de-vice beamline ID32. Journal of Electron Spectroscopy and Related Phenomena, 178179(0):258–267, May 2010.
21G. Panaccione, G. Cautero, M. Cautero, A. Fondacaro, M. Grioni, C.
Henri-quet, G. Monaco, M. Mulazzi, F. Offi, L. Paolasini, G. Paolicelli, P. Pittana, M. Sacchi, G. Stefani, and P. Torelli. Results and perspectives in hard x-ray photoemission spectroscopy (HAXPES) from solids. Nuclear Instruments and Methods in Physics Research Section B: Beam Interactions with Materials and Atoms, 246(1):106–111, May 2006.
23W. Fredriksson, S. Malmgren, T. Gustafsson, M. Gorgoi, and K. Edstrm. Full
depth profile of passive films on 316l stainless steel based on high resolution HAXPES in combination with ARXPS. Applied Surface Science, 258(15):5790– 5797, May 2012.
24Patrick S. Lysaght, Joel Barnett, Gennadi I. Bersuker, Joseph C. Woicik,
Daniel A. Fischer, Brendan Foran, Hsing-Huang Tseng, and Raj Jammy. Chem-ical analysis of HfO2/Si (100) film systems exposed to NH3 thermal processing.
25R Claessen, M Sing, M Paul, G Berner, A Wetscherek, A M¨uller, and W Drube.
Hard x-ray photoelectron spectroscopy of oxide hybrid and heterostructures: a new method for the study of buried interfaces. New Journal of Physics, 11(12):125007, December 2009.
26J. Rubio-Zuazo, E. Martinez, P. Batude, L. Clavelier, A. Chabli, and G.R.
Castro. Probing buried interfaces on Ge-based metal gate/high-κ stacks by hard x-ray photoelectron spectroscopy. Applied Surface Science, 257(7):3007– 3013, January 2011.
27Noelia Benito, Ramn Escobar Galindo, Juan Rubio-Zuazo, Germn R.
Cas-tro, and Carlos Palacio. High and low-energy x-ray photoelectron techniques for compositional depth profiles: destructive versus non-destructive methods.
Journal of Physics D: Applied Physics, 46(6):065310, February 2013.
28C. Weiland, P. Lysaght, J. Price, J. Huang, and J. C. Woicik. Hard x-ray
photo-electron spectroscopy study of As and Ga out-diffusion in In0.53Ga0.47As/Al2O3
film systems. Applied Physics Letters, 101(6):061602, August 2012.
29C. Weiland, A. K. Rumaiz, J. Price, P. Lysaght, and J. C. Woick. Passivation of
In0.53Ga0.47As/ZrO2 interfaces by AlN atomic layer deposition process. Journal
of Applied Physics, 114(3):034107, July 2013.
30Masakazu Baba, Keita Ito, Weijie Du, Tatsunori Sanai, Kazuaki Okamoto,
Kaoru Toko, Shigenori Ueda, Yoji Imai, Akio Kimura, and Takashi Suemasu. Hard x-ray photoelectron spectroscopy study on valence band structure of semi-conducting BaSi2.Journal of Applied Physics, 114(12):123702, September 2013. 31D. Gerlach, D. Wippler, R. G. Wilks, M. Wimmer, M. Lozac’h, R. F´elix,
S. Ueda, H. Yoshikawa, K. Lips, B. Rech, M. Sumiya, K. Kobayashi, M. Gorgoi, J. H¨upkes, and M. B¨ar. p-type a-Si:H/ZnO:Al and c-Si:H/ZnO:Al thin-film so-lar cell structures; a comparative hard x-ray photoelectron spectroscopy study.
IEEE Journal of Photovoltaics, 3(1):483–487, 2013.
OMeTAD molecular thin films when adding Li-TFSI. The Journal of Physical Chemistry C, 116(50):26300–26305, December 2012.
33Michael T. Brumbach and Joseph C. Woicik. HAXPES of protected ITO
surfaces at the buried P3HT/ITO interface. Surface and Interface Analysis,
34Tadao Shibuya, Masahiro Yoshinaka, Yukio Shimane, Futoshi Utsuno, Koki
Yano, Kazuyoshi Inoue, Eiji Ikenagab, Jung J. Kim, Shigenori Ueda, Masaaki Obata, and Keisuke Kobayashi. Electronic structural analysis of transparent In2O3ZnO films by hard x-ray photoelectron spectroscopy. Thin Solid Films,
518(11):3008–3011, March 2010.
35Masahiro Shibuta, Toyoaki Eguchi, Yoshio Watanabe, Jin-Young Son, Hiroshi
Oji, and Atsushi Nakajima. Probing buried organic-organic and metal-organic heterointerfaces by hard x-ray photoelectron spectroscopy. Applied Physics Letters, 101(22):221603, November 2012.
36S. Laureti, L. Del Bianco, B. Detlefs, E. Agostinelli, V. Foglietti, D. Peddis,
A.M. Testa, G. Varvaro, and D. Fiorani. Interface exchange coupling in a CoPt/NiO bilayer. Thin Solid Films, 543:162–166, September 2013.
37Ranjeeta Gupta, Ajay Gupta, Mukul Gupta, Parasmani Rajput, and Andrew
Wildes. Evolution of structural and magnetic properties of amorphous CoFeB film with thermal annealing.Journal of Applied Physics, 114(6):063903, August 2013.
38C. Caspers, M. Mller, A. X. Gray, A. M. Kaiser, A. Gloskovskii, C. S. Fadley,
W. Drube, and C. M. Schneider. Chemical stability of the magnetic oxide EuO directly on silicon observed by hard x-ray photoemission spectroscopy. Physical Review B, 84(20):205217, November 2011.
39A. M¨uller, A. Ruff, M. Paul, A. Wetscherek, G. Berner, U. Bauer, C. Praetorius,
K. Fauth, M. Przybylski, M. Gorgoi, M. Sing, and R. Claessen. Fe3O4 on
ZnO: A spectroscopic study of film and interface properties. Thin Solid Films, 520(1):368–373, October 2011.
40Mac C. Mugumaoderha, Robert Sporken, Jacques Ghijsen, and Jacques A.
Dumont. Physical chemistry of the Mn/ZnO (000¯1) interface probed by hard x-ray photoelectron spectroscopy. The Journal of Physical Chemistry C, 115(42):20603–20609, October 2011.
41Xeniya Kozina, Siham Ouardi, Benjamin Balke, Gregory Stryganyuk,
Ger-hard H. Fecher, Claudia Felser, Shoji Ikeda, Hideo Ohno, and Eiji Ikenaga. A nondestructive analysis of the b diffusion in Ta-CoFeB-MgO-CoFeB-Ta mag-netic tunnel junctions by hard x-ray photoemission. Applied Physics Letters, 96(7):072105, February 2010.
42Mykhailo Vorokhta, Ivan Khalakhan, Iwa Matolnov, Masaaki Kobata, Hideki
Yoshikawa, Keisuke Kobayashi, and Vladimir Matoln. Nanostructured PtCeO2
thin film catalyst grown on graphite foil by magnetron sputtering. Applied Surface Science, 267:119–123, February 2013.
43A. M. Kaiser, A. X. Gray, G. Conti, B. Jalan, A. P. Kajdos, A. Gloskovskii,
S. Ueda, Y. Yamashita, K. Kobayashi, W. Drube, S. Stemmer, and C. S. Fadley. Electronic structure of delta-doped La:SrTiO3 layers by hard x-ray
photoelec-tron spectroscopy. Applied Physics Letters, 100(26):261603, June 2012.
44Y. Y. Chu, Y. F. Liao, V. T. Tra, J. C. Yang, W. Z. Liu, Y. H. Chu, J. Y.
Lin, J. H. Huang, J. Weinen, S. Agrestini, K.-D. Tsuei, and D. J. Huang. Distribution of electronic reconstruction at the n-type LaAlO3/SrTiO3 interface
revealed by hard x-ray photoemission spectroscopy. Applied Physics Letters, 99(26):262101, December 2011.
45Reza Younesi, Sigita Urbonaite, Kristina Edstrm, and Maria Hahlin. The
cath-ode surface composition of a cycled LiO2 battery: A photoelectron spectroscopy
study. The Journal of Physical Chemistry C, 116(39):20673–20680, October 2012.
46S. Malmgren, K. Ciosek, M. Hahlin, T. Gustafsson, M. Gorgoi, H. Rensmo, and
com-47M. Sowinska, T. Bertaud, D. Walczyk, S. Thiess, M. A. Schubert, M.
Luko-sius, W. Drube, Ch Walczyk, and T. Schroeder. Hard x-ray photoelectron spectroscopy study of the electroforming in Ti/HfO2-based resistive switching
structures. Applied Physics Letters, 100(23):233509, June 2012.
48Abdul K. Rumaiz, C. Jaye, J. C. Woicik, Weigang Wang, D. A. Fischer,
J. Jordan-Sweet, and C. L. Chien. Boron migration due to annealing in CoFeB/MgO/CoFeB interfaces: A combined hard x-ray photoelectron spec-troscopy and x-ray absorption studies. Applied Physics Letters, 99(22):222502, November 2011.
49M. Minnekaev, K. Bulakh, A. Chouprik, W. Drube, P. Ershov, Yu.
Lebedin-skii, K. Maksimova, and A. Zenkevich. Structural, ferroelectric, electronic and transport properties of BaTiO3/Pt heterostructures grown on MgO(001).
Mi-croelectronic Engineering, 109:227–231, September 2013.
50Abdul K. Rumaiz, J. C. Woicik, G. A. Carini, D. P. Siddons, E. Cockayne,
E. Huey, P. S. Lysaght, D. A. Fischer, and V. Genova. Band alignment of atomic layer deposited HfO2 on clean and N-passivated germanium surfaces.
Applied Physics Letters, 97(24):242108–242108–3, December 2010.
51M. Gaowei, E. M. Muller, A. K. Rumaiz, C. Weiland, E. Cockayne, J.
Jordan-Sweet, J. Smedley, and J. C. Woicik. Annealing dependence of diamond-metal schottky barrier heights probed by hard x-ray photoelectron spectroscopy. Ap-plied Physics Letters, 100(20):201606, 2012.
52Xeniya Kozina, Gerhard H. Fecher, Gregory Stryganyuk, Siham Ouardi,
Benjamin Balke, Claudia Felser, Gerd Sch¨onhense, Eiji Ikenaga, Takeharu Sugiyama, Naomi Kawamura, Motohiro Suzuki, Tomoyuki Taira, Tetsuya Ue-mura, Masafumi Yamamoto, Hiroaki Sukegawa, Wenhong Wang, Koichiro Ino-mata, and Keisuke Kobayashi. Magnetic dichroism in angle-resolved hard x-ray photoemission from buried layers. Physical Review B, 84(5):054449, August 2011.
53Juan Rubio-Zuazo and German R. Castro. Beyond hard x-ray photoelectron
spectroscopy: Simultaneous combination with x-ray diffraction. Journal of Vacuum Science & Technology A, 31(3):031103, April 2013.
54Toyli Anniyev, Hirohito Ogasawara, Mathias P. Ljungberg, Kjartan T.
Wik-feldt, Janay B. MacNaughton, Lars-˚Ake N¨aslund, Uwe Bergmann, Shirlaine Koh, Peter Strasser, Lars G. M. Pettersson, and Anders Nilsson. Complemen-tarity between high-energy photoelectron and L-edge spectroscopy for probing the electronic structure of 5d transition metal catalysts. Physical Chemistry Chemical Physics, 12(21):5694–5700, May 2010.
55C. Papp, G. Conti, B. Balke, S. Ueda, Y. Yamashita, H. Yoshikawa, Y. S.
Urit-sky, K. Kobayashi, and C. S. Fadley. Nondestructive characterization of a TiN metal gate: Chemical and structural properties by means of standing-wave hard x-ray photoemission spectroscopy. Journal of Applied Physics, 112(11):114501, December 2012.
56S. Grebinskij, ˇS. Masys, S. Mickeviˇcius, V. Lisauskas, and V. Jonauskas. Ab
ini-tio and photoemission study of correlaini-tion effects in SrRuO3thin films.Physical
Review B, 87(3):035106, January 2013.
57S. Suga, A. Sekiyama, S. Imada, T. Miyamachi, H. Fujiwara, A. Yamasaki,
K. Yoshimura, K. Okada, M. Yabashi, K. Tamasaku, A. Higashiya, and T. Ishikawa. ∼8 keV photoemission of the metalinsulator transition system VO2. New Journal of Physics, 11(10):103015, October 2009.
58W. Meissner and B. Voigt. Messungen mit hilfe von fl¨ussigem helium XI
widerstand der reinen metalle in tiefen temperaturen. Annalen der Physik, 399(8):892–936, January 1930.
59Jun Kondo. Resistance minimum in dilute magnetic alloys. Progress of
Theo-retical Physics, 32(1):37–49, July 1964.
Taniguchi. Electronic structure of kondo lattice compounds YbNi3X9 (X =
al, ga) studied by hard x-ray spectroscopy. Physical Review B, 86(11):115114, September 2012.
61M. Matsunami, A. Chainani, M. Taguchi, R. Eguchi, Y. Takata, M. Oura,
M. Yabashi, K. Tamasaku, Y. Nishino, T. Ishikawa, M. Kosaka, and S. Shin. Photoemission evidence for valence fluctuations and Kondo resonance in YbAl2.
arXiv:1206.1689 [cond-mat], June 2012. J. Phys. Soc. Jpn. 81 (2012) 073702.
62L. Moreschini, C. Dallera, G. Monaco, G. Panaccione, A. Fondacaro, G.
Pao-licelli, P. Torelli, and M. Grioni. Comparison of bulk-sensitive spectroscopic probes of Yb valence in Kondo systems. Physical Review B, 75(3):035113, Jan-uary 2007.
63J. Yamaguchi, A. Sekiyama, M. Y. Kimura, H. Sugiyama, Y. Tomida, G.
Fun-abashi, S. Komori, T. Balashov, W. Wulfhekel, T. Ito, S. Kimura, A. Higashiya, K. Tamasaku, M. Yabashi, T. Ishikawa, S. Yeo, and S. Suga. Different evolution of intrinsic gap in kondo semiconductors SmB6 and YbB12. arXiv:1002.2530
[cond-mat], February 2010.
64Kahng Dawon. Electric field controlled semiconductor device, August
1963. U.S. Classification 323/349, 330/277, 257/288, 438/586, 327/581; International Classification H01L23/29, H01L29/00; Cooperative Classifi-cation H01L29/00, H01L2924/3011, H01L23/291; European ClassifiClassifi-cation H01L23/29C, H01L29/00.
65Gordon E. Moore. Cramming more components onto integrated circuits.
Elec-tronics magazine, 38(8), 1965.
66International technology roadmap for semiconductors. pages 3–4. 2011. 67Moore’s law, February 2014. Page Version ID: 595241510.
68Wolfgang Arden, Michel Brillouet, Patrick Cogez, Mart Graef, Bert Huizing,
and Reinhard Mahnkopf. More than moore.
69Dilute III-V Nitride Semiconductors and Material Systems - Physics and
70Robert M. Wallace, Paul C. McIntyre, Jiyoung Kim, and Yoshio Nishi. Atomic
layer deposition of dielectrics on Ge and III-V materials for ultrahigh perfor-mance transistors. MRS Bulletin, 34(07):493–503, 2009.
71T.D. Lin, H. C. Chiu, P. Chang, L. T. Tung, C.P. Chen, M. Hong,
J. Kwo, W. Tsai, and Y.C. Wang. High-performance self-aligned inversion-channel In0.53Ga0.47As metal-oxide-semiconductor field-effect-transistor with
Al2O3/Ga2O3(Gd2O3) as gate dielectrics. Applied Physics Letters,
72Y. Xuan, Y.Q. Wu, H.C. Lin, T. Shen, and P.D. Ye. Submicrometer
inversion-type enhancement-mode InGaAs MOSFET with atomic-layer-deposited Al2O3
as gate dielectric. IEEE Electron Device Letters, 28(11):935–938, 2007.
73S. Koveshnikov, N. Goel, P. Majhi, H. Wen, M.B. Santos, S. Oktyabrsky,
V. Tokranov, R. Kambhampati, R. Moore, F. Zhu, J. Lee, and W. Tsai. In0.53Ga0.47As based metal oxide semiconductor capacitors with atomic layer
deposition ZrO2 gate oxide demonstrating low gate leakage current and
equiv-alent oxide thickness less than 1 nm. Applied Physics Letters, 92(22):222904– 222904–3, 2008.
74N. Goel, D. Heh, S. Koveshnikov, I. Ok, S. Oktyabrsky, V. Tokranov, R.
Kamb-hampatic, M. Yakimov, Y. Sun, P. Pianetta, C.K. Gaspe, M.B. Santos, J. Lee, S. Datta, P. Majhi, and W. Tsai. Addressing the gate stack challenge for high mobility InxGa1−xAs channels for n-FETs. InElectron Devices Meeting, 2008.
IEDM 2008. IEEE International, pages 1–4, 2008.
75N. Goel, P. Majhi, C. O. Chui, W. Tsai, D. Choi, and J. S. Harris.
In-GaAs metal-oxide-semiconductor capacitors with HfO2 gate dielectric grown
by atomic-layer deposition. Applied Physics Letters, 89(16):163517, October 2006.
76D. Shahrjerdi, Thomas Rotter, G. Balakrishnan, Diana Huffaker, E. Tutuc, and
77M. L. Huang, Y. C. Chang, C. H. Chang, Y. J. Lee, P. Chang, J. Kwo, T. B.
Wu, and M. Hong. Surface passivation of III-V compound semiconductors using atomic-layer-deposition-grown Al2O3. Applied Physics Letters, 87(25):252104,
78Sylwia Klejna and Simon D. Elliott. First-principles modeling of the clean-up of
native oxides during atomic layer deposition onto III-V substrates. The Journal of Physical Chemistry C, 116(1):643–654, January 2012.
79M.K. Hudait, G. Dewey, S. Datta, J.M. Fastenau, J. Kavalieros, W. K. Liu,
D. Lubyshev, R. Pillarisetty, W. Rachmady, M. Radosavljevic, T. Rakshit, and R. Chau. Heterogeneous integration of enhancement mode In0.7Ga0.3As
quan-tum well transistor on silicon substrate using thin (less than 2 nm) composite buffer architecture for high-speed and low-voltage ( 0.5 V) logic applications. In
Electron Devices Meeting, 2007. IEDM 2007. IEEE International, pages 625– 628, 2007.
80Niamh Waldron, Gang Wang, Ngoc D. Nguyen, Tommaso Orzali, Clement
Merckling, Guy Brammertz, Patrick Ong, Gillis Winderickx, Geert Hellings, Geert Eneman, Matty Caymax, Marc Meuris, Naoto Horiguchi, and Aaron Thean. Integration of InGaAs channel n-MOS devices on 200 mm Si wafers using the aspect-ratio-trapping technique. ECS Transactions, 45(4):115–128, April 2012.
81Shinichi Takagi, Masafumi Yokoyama, Hideki Takagi, Yuji Urabe, Tetsuji
Ya-suda, Hisashi Yamada, Masahiko Hata, and Mitsuru Takenaka. (invited) III-V-On-Insulator MOSFETs on Si substrates fabricated by direct bonding tech-nique. ECS Transactions, 33(4):359–370, October 2010.
82Masafumi Yokoyama, Ryo Iida, Yuki Ikku, Sanghyeon Kim, Hideki Takagi,
Tet-suji Yasuda, Hisashi Yamada, Osamu Ichikawa, Noboru Fukuhara, Masahiko Hata, Mitsuru Takenaka, and Shinichi Takagi. Formation of III-V-on-insulator structures on Si by direct wafer bonding. Semiconductor Science and Technol-ogy, 28(9):094009, September 2013.
83M. Radosavljevic, B. Chu-Kung, S. Corcoran, G. Dewey, M.K. Hudait, J.M.
Fastenau, J. Kavalieros, W. K. Liu, D. Lubyshev, M. Metz, K. Millard, N. Mukherjee, W. Rachmady, U. Shah, and R. Chau. Advanced high-κ gate dielectric for high-performance short-channel In0.7Ga0.3As quantum well field
ef-fect transistors on silicon substrate for low power logic applications. InElectron Devices Meeting (IEDM), 2009 IEEE International, pages 1–4, 2009.
84Guy Brammertz, H. C. Lin, Koen Martens, Ali-Reza Alian, C. Merckling, Julien
Penaud, David Kohen, W.-E. Wang, S. Sioncke, A. Delabie, Marc Meuris, Matty R. Caymax, and Marc Heyns. Electrical properties of III-V/oxide inter-faces. ECS Transactions, 19(5):375–386, May 2009.
85B. Brennan, M. Milojevic, C.L. Hinkle, F.S. Aguirre-Tostado, G. Hughes, and
R.M. Wallace. Optimisation of the ammonium sulphide (NH4)2S passivation
process on In0.53Ga0.47As. Applied Surface Science, 257(9):4082–4090, February
86C. L. Hinkle, M. Milojevic, B. Brennan, A. M. Sonnet, F. S. Aguirre-Tostado,
G. J. Hughes, E. M. Vogel, and R. M. Wallace. Detection of Ga suboxides and their impact on III-V passivation and Fermi-level pinning. Applied Physics Letters, 94(16):162101, April 2009.
87L. Lin and J. Robertson. Defect states at III-V semiconductor oxide interfaces.
Applied Physics Letters, 98(8):082903–082903–3, February 2011.
88Achuthan-Bhat. Fundamentals Of Semicon Dev. Tata McGraw-Hill Education,
89 OConnor, B. Brennan, V. Djara, K. Cherkaoui, S. Monaghan, S. B. Newcomb,
R. Contreras, M. Milojevic, G. Hughes, M. E. Pemble, R. M. Wallace, and P. K. Hurley. A systematic study of (NH4)2S passivation (22%, 10%, 5%, or
1%) on the interface properties of the Al2O3/In0.53Ga0.47As/InP system for
n-type and p-n-type In0.53Ga0.47As epitaxial layers. Journal of Applied Physics,
on a GaAs substrate with ZrO2 high-κ dielectrics. Japanese Journal of Applied
Physics, 47(5):3441–3443, 2008.
91Alessandro Molle, Guy Brammertz, Luca Lamagna, Marco Fanciulli, Marc
Meuris, and Sabina Spiga. Ge-based interface passivation for atomic layer de-posited La-doped ZrO2 on III-V compound (GaAs, In0.15Ga0.85As) substrates.
Applied Physics Letters, 95(2):023507, July 2009.
92M. Akazawa and H. Hasegawa. High-κ Al
2O3 MOS structures with Si interface
control layer formed on air-exposed GaAs and InGaAs wafers. Applied Surface Science, 256(19):5708–5713, July 2010.
93S. Koveshnikov, W. Tsai, I. Ok, J. C. Lee, V. Torkanov, M. Yakimov, and
S. Oktyabrsky. Metal-oxide-semiconductor capacitors on GaAs with high-κ
gate oxide and amorphous silicon interface passivation layer. Applied Physics Letters, 88(2):022106, January 2006.
94Zuoguang Liu, Sharon Cui, Pini Shekhter, Xiao Sun, Lior Kornblum, Jie Yang,
Moshe Eizenberg, K. S. Chang-Liao, and T. P. Ma. Effect of H on inter-face properties of Al2O3/In0.53Ga0.47As.Applied Physics Letters, 99(22):222104,
95G. Brammertz, H. C. Lin, K. Martens, D. Mercier, C. Merckling, J. Penaud,
C. Adelmann, S. Sioncke, W. E. Wang, M. Caymax, M. Meuris, and M. Heyns. Capacitance-voltage characterization of GaAs-oxide interfaces. Journal of The Electrochemical Society, 155(12):H945–H950, December 2008.
96S. Nishida, H. Uchida, and S. Kaneko. A new self-aligned a-SI TFT using
ion doping and chromium silicide formation. MRS Online Proceedings Library, 219:null–null, 1991.
97Yue Kuo. Thin Film Transistor Technologies: Proceedings of the Fourth
Sym-posium on Thin Film Transistor Technologies. The Electrochemical Society, 1999.
98Mulpuri V. Rao. Ion implantation in III-V compound semiconductors. Nuclear
Instruments and Methods in Physics Research Section B: Beam Interactions with Materials and Atoms, 79(14):645–647, June 1993.
99Xingui Zhang, Huaxin Guo, Xiao Gong, Qian Zhou, You-Ru Lin, Hau-Yu Lin,
Chih-Hsin Ko, Clement H. Wann, and Yee-Chia Yeo. In0.7Ga0.3As channel
n-MOSFET with self-aligned Ni-InGaAs source and drain. Electrochemical and Solid-State Letters, 14(2):H60–H62, February 2011.
100Ivana, Jisheng Pan, Zheng Zhang, Xingui Zhang, Huaxin Guo, Xiao Gong, and
Yee-Chia Yeo. Photoelectron spectroscopy study of band alignment at interface between Ni-InGaAs and In0.53Ga0.47As. Applied Physics Letters, 99(1):012105,
101L. Czornomaz, M. El Kazzi, M. Hopstaken, D. Caimi, P. Mchler, C. Rossel,
M. Bjoerk, C. Marchiori, H. Siegwart, and J. Fompeyrine. CMOS compat-ible self-aligned s/d regions for implant-free InGaAs MOSFETs. Solid-State Electronics, 74:71–76, August 2012.
102Ivana, Yong Lim Foo, Xingui Zhang, Qian Zhou, Jisheng Pan, Eugene Kong,
Man Hon Samuel Owen, and Yee-Chia Yeo. Crystal structure and epitaxial relationship of Ni4InGaAs2 films formed on InGaAs by annealing. Journal of
Vacuum Science & Technology B: Microelectronics and Nanometer Structures, 31(1):012202, 2013.
Theory and Experimental
The principal technique used in this report is x-ray photoelectron spectroscopy and its high energy variant, hard x-ray photoelectron spectroscopy (HAXPES). In this section the theoretical and experimental basis of these, and other relevant techniques will be explained. The experimental systems used in this report will also be described.
X-ray Photoelectron Spectroscopy
XPS is based on the photoelectric effect,1 which predicts that when a photon strikes an atom one of three outcomes occurs:
1. The photon does not interact and passes through undisturbed.
2. The photon may interact with an electron and pass all of its energy to that electron causing it to be emitted from the atom, as seen in figure 2.1.
Figure 2.1: Emission of an electron from an atomic orbital due to the photoelectric effect.
3. The photon can be scattered upon interaction with an electron.
The second process is the basis of XPS, as it is these emitted electrons which are measured.
According to the photoelectric effect, no electron emission will occur unless the incident photons are of equal or greater frequency than the threshold frequency specific to the elements being studied. Once this condition is met, the number of emitted electrons is proportional to the intensity of the incident photons. The kinetic energy (KE) of the emitted electrons is directly proportional to the fre-quency of the photons used. This photoemission process is extremely rapid (10−16 seconds). The relationship is succinctly described by the Einstein equation:2
BE =hν−KE, (2.1)
where BE is the binding energy of the emitted photoelectron in the atom, h is Planck’s constant and ν is the frequency of the incident photons.